### Delft University of Technology

### Phonon broadening in high entropy alloys

### Kormann, Fritz; Ikeda, Yuji; Grabowski, Blazej; Sluiter, Marcel

### DOI

### 10.1038/s41524-017-0037-8

### Publication date

### 2017

### Document Version

### Final published version

### Published in

### npj Computational Materials

### Citation (APA)

### Kormann, F., Ikeda, Y., Grabowski, B., & Sluiter, M. (2017). Phonon broadening in high entropy alloys. npj

### Computational Materials, 3, [36]. https://doi.org/10.1038/s41524-017-0037-8

### Important note

### To cite this publication, please use the final published version (if applicable).

### Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

### ARTICLE

**OPEN**

## Phonon broadening in high entropy alloys

Fritz Körmann 1_{, Yuji Ikeda}2

_{, Blazej Grabowski}3

_{and Marcel H. F. Sluiter}1

Refractory high entropy alloys feature outstanding properties making them a promising materials class for next-generation high-temperature applications. At high high-temperatures, materials properties are strongly affected by lattice vibrations (phonons). Phonons critically inﬂuence thermal stability, thermodynamic and elastic properties, as well as thermal conductivity. In contrast to perfect crystals and ordered alloys, the inherently present mass and force constantﬂuctuations in multi-component random alloys (high entropy alloys) can induce signiﬁcant phonon scattering and broadening. Despite their importance, phonon scattering and broadening have so far only scarcely been investigated for high entropy alloys. We tackle this challenge from a theoretical perspective and employ ab initio calculations to systematically study the impact of force constant and massﬂuctuations on the phonon spectral functions of 12 body-centered cubic random alloys, from binaries up to 5-component high entropy alloys, addressing the key question of how chemical complexity impacts phonons. Weﬁnd that it is crucial to include both mass and force constantﬂuctuations. If one or the other is neglected, qualitatively wrong results can be obtained such as artiﬁcial phonon band gaps. We analyze how the results obtained for the phonons translate into thermodynamically integrated quantities, speciﬁcally the vibrational entropy. Changes in the vibrational entropy with increasing the number of elements can be as large as changes in the conﬁgurational entropy and are thus important for phase stability considerations. The set of studied alloys includes MoTa, MoTaNb, MoTaNbW, MoTaNbWV, VW, VWNb, VWTa, VWNbTa, VTaNbTi, VWNbTaTi, HfZrNb, HfMoTaTiZr.

npj Computational Materials (2017) 3:36 ; doi:10.1038/s41524-017-0037-8

INTRODUCTION

High entropy alloys (HEA) are of great technological interest due
to their excellent mechanical1, 2 and electronic properties.3
Refractory HEAs, such as e.g. bcc NbMoTaW, possess extraordinary
mechanical properties, comparable to current state-of-the-art
nickel-based superalloys.2, 4–6 This makes them promising
candidates for next-generation high-temperature applications.
The design of materials for extreme temperature environments
requires an accurate knowledge of phase stabilities,
thermody-namic properties and thermal conductivity,7all of which are linked
intrinsically to lattice vibrations, i.e. phonons.8, 9 _{Accurate}
modeling of phonon excitations and their interactions plays
therefore a decisive role in the design, exploration and
optimiza-tion of such materials.

Phonons can be altered by nano-structural features (e.g., nanoparticles, nanowires),10, 11 they interact with themselves (i.e., phonon-phonon interactions)9and with chemical disorder, a key feature of HEAs.12–14The interaction with chemical disorder can lead to signiﬁcant phonon scattering and broadening, if elements of considerable mass difference are involved. In addition to the mass disorder, the locally distinct chemical environments in HEAs can induce force constant variations that also modify the phonon spectral distribution. These force constant variations may be enhanced by local lattice distortions that are known to be important in HEAs.13–17

The large compositional space inherent to HEAs offers the possibility to tune phonon broadening by adjusting the chemical complexity via variation of the relative fractions of the constituent elements and the total number of elements. The mass and force

constant induced scattering processes could be, for example, used to modify systematically thermal conductivity (inversely propor-tional to phonon bandwidth). This is of particular interest for HEAs that were recently suggested as candidates for thermoelectric18,19 or heat shield materials.7

Tuning chemical complexity in HEAs has been employed to
tailor electron scattering and electronic properties20,21_{aiming at}
improved radiation resistant materials. Similar studies on disorder
induced phonon scattering and phonon broadening in HEAs are
so far lacking. Previous works addressing phonons in disordered
alloys have been mostly limited to binaries.22–27A few works have
been devoted to vibrational properties of multi-component
alloys,16, 28–31 but were mainly focused on integrated quantities
such as the phonon density of states28 or thermodynamic
properties such as lattice speciﬁc heat, typically derived from
simpliﬁed Debye-like models.29, 30 Phonon spectra and in
particular mass and force constant induced phonon broadening
remain unexplored.

Therefore, we have performed an extensive ﬁrst-principles study to evaluate phonon broadening for 12 different body-centered cubic (BCC) refractory random alloys, from binaries up to 5-component high entropy alloys. Our set of alloys includes in particular the 4-component NbMoTaW, NbTaTiV, NbTaVW, and 5-component NbMoTaWV, NbTaTiVW, HfMoTaTiZr alloys, which attracted attention recently.4, 16, 30, 32–34 On the basis of our results, we address the following fundamental questions: How strongly are phonon spectra affected in high entropy alloys by chemical disorder induced scattering? What is the detailed contribution due to mass and force constant ﬂuctuations? Are both equally important or could one or the other be neglected?

Received: 30 April 2017 Revised: 11 July 2017 Accepted: 18 July 2017 1

Materials Science and Engineering, Delft University of Technology, 2628 CD Delft, The Netherlands;2

Center for Elements Strategy Initiative for Structural Materials, Kyoto University, Kyoto 606-8501, Japan and3

Computationals Materials Design, Max-Planck-Institut für Eisenforschung GmbH, 40237 Düsseldorf, Germany Correspondence: Fritz Körmann (f.h.w.kormann@tudelft.nl) or Yuji Ikeda (ikeda.yuji.6m@kyoto-u.ac.jp)

And what is the role of the number of constituent elements for phonon broadening?

RESULTS

Figure 1 shows the computed phonon spectra for two sets of alloys, namely MoTa, MoTaNb, MoTaNbW, MoTaNbWV in (a)–(d) and VW, VWNb, VWNbTa, VWNbTaTi in (g)–(j) (added elements in bold), i.e., starting with binaries, moving to ternaries, then quaternaries, and ﬁnally to the ﬁve-component quinaries. This strategy of adding one element after the other allows us to study systematically the impact of the total number of principal elements on the phonon broadening. For all considered alloys, the long-wavelength limit (region close to Γ) is unaffected, i.e., no broadening is visible and the spectral function is sharply peaked as exempliﬁed in the two 3D insets (e) and (f) for MoTaNbW and MoTaNbWV. This long-wavelength behavior is a consequence of the Rayleigh law (~ω4) for impurity scattering.35For the mid- and high-frequency region (above ~ 4 THz), the broadening turns out to be very strong for all alloys, reaching widths of up to a few THz. Inspecting theﬁrst sequence of alloys (Figs.1a–d), the broadening

of the 4- and 5-component alloy spectra appears to be larger compared to the 2- and 3-component ones as exempliﬁed by the grey arrows at the H-point. This dependence is even better visible in the upper panel of Fig.2where the spectral function is drawn for the H-point. The impact of the number of components is qualitatively different for the second alloy series (Figs.1g–j), where

a phonon band gap appears for the phonon spectrum of VW around the H-point (grey dashed lines and arrow). This band gap disappears when more elements are added and the overall broadening is slightly contracted.

To analyze the observed behavior we will proceed in several steps, starting with a comparison to the most simpliﬁed approximation of chemical disorder. For that purpose we derived the phonon spectra based on the virtual-crystal approximation (VCA, black solid lines in Fig.1and black dashed lines in Fig.2), where we replaced the force constants with averaged values according to the crystal symmetries (i.e. by not distinguishing the different constituents) and the atomic masses with averaged

masses over the constituents. In the long-wavelength limit and for frequencies below ~ 4 THz the averaged spectra agree very well with the full calculation. However, for frequencies above ~ 4 THz, where the broadening sets in, the averaged dispersions fail in capturing the correct physics. Clearly, due to the averaging procedure broadening cannot be described. Moreover, the averaged dispersions do not match well in position with the corresponding (broadened) peaks in the full dispersion. The discrepancy is most obvious for VW where the averaged dispersion falls into the band gap region of the full calculation. We conclude that the VCA is a too simpliﬁed approximation. Similar observations have been recently made for face-centered cubic (FCC) random FePt alloys.36

The effective single-species approximation neglects mass ﬂuctuations. A convenient quantity to characterize the latter is the mass-ﬂuctuation phonon scattering parameter,35

ΓM¼ X ici Mi M 2 =M2 ; (1)

where ciand Midenote the concentration and atomic mass of the

i-th component and M the averaged mass of the alloy. Within the original Klemens model,35 ΓM is proportional to the inverse

relaxation time, which is often associated with the overall phonon broadening. We therefore employ our computed spectral func-tions to investigate a possible relafunc-tionship.

The scattering parameter, ΓM, for theﬁrst alloy series in Fig.1

upper panel is 0.09, 0.11, 0.10 and 0.19. The minor variation ofΓM

between the 2-, 3-, and 4-component alloys (ΓM≈ 0.1) seems to be

inconsistent with our observation above that the 4-component alloy (together with the 5-component one) reveals a more broadened spectrum than the 2- and 3-component ones. Inspecting the second alloy series, whereΓMvaries as 0.32, 0.26,

0.20, 0.29, substantiates the conclusion thatΓMalone cannot cover

all aspects of phonon broadening. The 2- and 5-component alloys, i.e. VW and VWNbTaTi, reveal qualitatively different phonon broadening although their ΓM parameters are similar (0.32 vs.

0.29). The reason that theΓMparameter is insufﬁcient to capture

all the complexity of the broadening is force constantﬂuctuations that modify the mass inducedﬂuctuations.

Binary Ternary Quaternary Quinary

(g) (h) (i) (j) (a) (b) (c) (d)

(e) (f)

Fig. 1 Broadening of phonon spectra with increasing number of constituent elements: From binaries to 5-component high entropy alloys. The added element for each alloy from left to right is shown in bold. Phonon spectra derived by employing averaged force constants and masses are shown for comparison as black solid lines. Mass-ﬂuctuation scattering parameters ΓM(described in the main text) are shown for

each alloy. Insets e and f provide 3D representations of the long-wavelength phonon spectra for MoTaNbW and MoTaNbWV Phonon broadening in high entropy alloys

F Körmann et al.

2

In order to separate the impact of mass and force constant ﬂuctuations, we derived partially averaged phonon spectra with the averaging performed only over the force constants leaving the massﬂuctuations unaffected. Subsequently, we applied a recently introduced projection procedure37 that resolves the contribution into the different pair interactions (Mo-Mo, Mo-Ta, etc.). The results for the MoTaNbWV series at the H-point are shown in the lower panel of Fig.2. The H-point is particularly convenient because, for a one-atomic or an averaged bcc bulk system, only a single frequency mode is present enabling an unbiased analysis of the broadening without intervention from other modes. Taking only the mass ﬂuctuations into account all element-projected con-tributions to the spectral functions can be directly related to their individual atomic masses. Generally, the lower the atomic mass the higher the frequency and vice versa. For example, Ta has a mass of 181 u and its spectral function (red) is placed in a region of about 4 to 5 THz, shifting somewhat down as the number of elements is increased. Mo is signiﬁcantly lighter with 96 u and its spectral function (blue) is in the range of 6 to 7 THz. Such a mass analysis makes a straightforward interpretation of the observedΓM

parameter dependence possible: The 2-, 3- and 4-component alloys can be considered as binary or quasi-binary, due to the overlap of some of the atomic masses, thus justifying the similar

ΓM≈ 0.1. It is only the 5-component alloy where a “new” mass of

51 u is introduced. This renders the alloy a quasi-ternary and increases ΓM to 0.19. The spectral functions involving mass

ﬂuctuations only (lower panel of Fig.2) are nicely consistent with this analysis. However, the full spectral functions (upper panel) are quite different and this is caused by force constantﬂuctuations.

To explain how the force constantﬂuctuations modify the mass induced broadening, we focus on the VW alloy where the effect is strongest. Figure3a shows the partially averaged spectral function for VW along the high symmetry directions. The phonon band gap is very large, from about 5 to 8 THz at the H point, due to the signiﬁcant mass difference between V (51 u) and W (184 u). Figure3b also shows a partially averaged spectral function. This time however, the massﬂuctuations are averaged out leaving the force constant ﬂuctuations unaffected. Although the resulting broadening is smaller than the one caused by the mass ﬂuctuations, it is still signiﬁcant with a width of about 3 THz. Such a signiﬁcant impact of force constant ﬂuctuations on the phonon broadening is generally found for the alloys studied here (seeSupplementary Information). Inspecting the complete spec-tral function including both mass and force constantﬂuctuations (Fig. 3c) reveals that the phonon band gap and the overall broadening are contracted with respect to the spectral function

Fig. 3 Impact of mass ﬂuctuations and force constant ﬂuctuations on the phonon broadening of the binary VW alloy. a Phonon spectra including only massﬂuctuations (averaged force constants), b phonon spectra including only force constant ﬂuctuations (averaged masses), and c phonon spectra including both mass and force constantﬂuctuations. Phonon spectra derived by employing averaged force constants and averaged masses are shown for comparison (black solid lines)

0 0.2 0.4 0.6 Spectral function (THz-1) 0 0.4 0.8 1.2 Spectral function (THz-1) 0 0.5 1 1.5 2 2.5 Spectral function (THz-1) 0 1 2 3 Spectral function (THz-1) 0 3 6 9 12 Frequency (THz)

Binary Ternary Quaternary Quinary

0 1 2 0 1 2 3 4 0 2 4 6 0 2 4 6 8 3 4 5 6 7 8 Frequency (THz)

MoTa MoNbTa MoNbTaW MoNbTaVW

Mass only Full Mo-Mo 96 u Ta-Ta 181 u V-V 51 u W-W 184 u Nb-Nb 93 u

binary binary ternary

*M *= 0.09 *M *= 0.11 *M *= 0.10 *M *= 0.19

average full

(e) (f) (g) (h) (a) (b) (c) (d)

Fig. 2 a-d: Full spectral functions of the ﬁrst alloy series (MoTa to MoNbTaVW) at the H-point. The dashed lines represent the spectral function (delta peaks) employing averaged force constants and masses. e–h: Spectral functions at the H-point projected on elemental pairs (Mo-Mo blue solid lineswith blue shading, Ta-Ta red solid lines with red shading, Nb-Nb dark violet dashed lines, W-W black dashed lines, and V-V green solid lineswith green shading) including only massﬂuctuations (averaged force constants)

with massﬂuctuations only. Similar ﬁndings have been reported for random FCC NiPt and CuAu alloys.22–24 Our results indicate that such counteractions are also present in multicomponent alloys.

In order to substantiate this ﬁnding, we focus in Figs.4a, b on the H-point. Figure4a emphasizes the phonon band gap when only massﬂuctuations are considered and clariﬁes that the lower peak is originating from vibrations of W (184 u) and the upper peak from vibrations of V (51 u). Figure4b shows that considering only force constant ﬂuctuations the two elements switch positions, V-V interactions are responsible for the lower and W-W interactions for the upper peak. This suggests that the lighter element V has smaller force constants and the heavier W has larger force constants. As a consequence, the force constants counteract the mass induced splitting of the spectral function contracting the band gap and the overall broadening. The resulting full spectral function is shown in Fig. 4a by the grey line. In contrast to the masses, for the force constants the mutual V-W interactions are very important (purple line in Fig.4b). They lead to a strong damping of the lower-frequency peak and an enhancement of the higher-frequency peak in the ﬁnal, full spectral function. Similar negative contributions to the spectral function of the mutual interactions have been found and discussed for Cu-Au recently.37

The mass ﬂuctuation induced broadening and splitting of the spectral functions can be rather straightforwardly analyzed and understood in terms of the atomic masses, as illustrated above for the MoTaNbWV series (Fig.2, lower panel). In contrast, the nature of force constantﬂuctuations is, in general, much more obscure. Such force constant ﬂuctuations are generated from the locally different chemical environments, which can be further modiﬁed by the variation of bond lengths (local lattice distortion). Often,

however, the main contribution is given by the nearest neighbor force constants and we have therefore investigated this possibility for the present alloys. Speciﬁcally, we have computed spectral functions excluding all force constants but the ones with the nearest neighbors. The results (shown in the Supplementary Information) reveal that many features of the phonon spectra and broadening can be observed in these reduced nearest-neighbor calculations, but longer-ranged interactions are needed for quantitative predictions. An example of theﬁrst nearest neighbor force constants is given in Figs.4c, d. Consistent with the above discussion, the V-V interactions reveal smaller force constants than the W-W ones. The relative peak positions for the V-V and W-W force constant distributions in Fig. 4d clearly correlate with the related projections of the spectral functions due to the force-constantﬂuctuations shown in Fig.4b.

The relationship between mass and force constantﬂuctuations is a general phenomenon for the studied alloys. Figure 5

exempliﬁes this relationship for the 5-component alloys. It shows the mean value of the computed magnitude of nearest-neighbor force constants of all pairs in the 5-component alloys versus the atomic masses. In addition to the already discussed NbTaTiVW and MoNbTaVW alloys, the HfMoTaTiZr alloy38 has been included, motivated by recent interest38 sparked by yield strengths comparable to current state-of-the-art superalloys. Note that the ternary HfNbZr sub-system is discussed in the Supplementary Information. The solid lines represent second order polynomialﬁts to the computed data and they reveal a clear relation of the masses and force constants for all quinaries. The larger the atomic masses the larger are the computed force constants. This relationship is the underlying reason for the partial compensation of the massﬂuctuations by the force constant ﬂuctuations.

Fig. 4 Projected W-W (red lines) and V-V (blue lines) as well as V-W (purple lines) contributions to the spectral functions if only a mass and b only force constantﬂuctuations are included. In a the total spectral function is shown in grey. c Absolute values of the x-x components of the nearest-neighbor force constants of W-W, V-W and V-V and d the corresponding force constant density of states. The relative peak positions of the force constant density of states in d correlate with the force constantﬂuctuation contributions to the spectral functions in b and counteract the mass disorder induced contributions to the spectral functions in a. Details are given in the text

50 100 150 200

Mass (atomic units) 0.4

0.8 1.2 1.6

1NN force constant (eV/Å

2)

MoNbTaVW

50 100 150 200

Mass (atomic units) 0.4

0.8 1.2

NbTaTiVW

50 100 150 200

Mass (atomic units) 0.4

0.8 1.2

HfMoTaTiZr (a) (b) (c)

Fig. 5 Absolute values of the x-x components of the nearest-neighbor force constants of the respective 15 elemental pairs in the 5-component alloys a MoNbTaVW, b NbTaTiVW, and c HfMoTaTiZr. The force constants are shown versus the square-root of the mass product of the atomic pairs including the standard deviation as obtained from the force constant distributions shown in Fig.4c. The lines are second order polynomialﬁts to the data. The atomic mass correlates with the computed force constants: the larger the mass, the larger the force constants. This correlation causes a partial compensation of the mass ﬂuctuation induced phonon broadening by the force constant ﬂuctuations

Phonon broadening in high entropy alloys F Körmann et al.

4

An important tool in the above analysis of the phonon spectral function was the decomposition into the contributions of the various element-element interactions. For the VW binary the projection procedure37resulted in partial spectral functions for V-V, V-W, and W-W interactions. The virtue of such a decomposition is the close correspondence to force constants between the elements as exploited above. However, for multicomponent alloys the analysis and interpretation based on pair interactions including cross-terms (such as V-W) becomes increasingly cumbersome. For a 5-component alloy already 15 various element-element interactions are present. We therefore propose an alternative projection scheme that allows one to map the total phonon spectral function onto single elements (not element-element pairs). Within this projection scheme, the unfolded partial spectral function for each element X is obtained as

AX _{k}
k; ω

ð Þ ¼X_{J}wXðK; JÞ wkkðK; JÞ δ ω ω K; J½ ð Þ; (2)
where K is a general wave vector, kka wave vector in the ﬁrst

Brillouin zone of the underlying crystal structure (here bcc), J a phonon mode index,ω(K, J) the phonon frequency at K and J, and wX(K, J) and wkkðK; JÞ corresponding weights given by:

wXðK; JÞ ¼ ^P X ~v K; Jð Þ h i 0 2; wkkðK; JÞ ¼ ^P kk ~v K; Jð Þ h i 0 2: (3)

Here,~v K; Jð Þ is the phonon eigenmode at K and J, and ^PX_{and ^}_{P}kk
are projection operators onto the species X and the wave vector
kk. The subscript“0” indicates that the norms are taken for the

original unit cell of the supercell model. A detailed derivation of the equations and explicit expressions for the projection operators are given in theSupplementary Information.

The above projection scheme allows us to decompose the full phonon spectra into the individual contributions of each element without requiring cross-terms, thus facilitating the interpretation. To demonstrate the projection scheme we consider the second alloy series in Fig.1, i.e. VW to VWNbTaTi, but now resolved into the individual contributions of each chemical element. The results are shown in Fig.6with the full spectra in theﬁrst column and their individually resolved contributions in the corresponding rows. Note that the partial phonon spectral functions include both mass and force constantﬂuctuations. The decomposition clearly reveals that the highest frequencies for each alloy are predomi-nantly determined by the lightest elements whereas the heavier ones determine the low-frequency parts. This is fully consistent with our ﬁndings above. We further see that, apart from the reduced concentration when going from top to bottom, the element speciﬁc contributions turn out to be rather independent of the actual alloy. This may open an efﬁcient route for predicting phonon spectra of alloys that have not yet been explored.

So far in this section, we have focused on the impact of chemical disorder on spectral functions, i.e., on the detailed wavevector-resolved frequency-dependence of the vibrational spectrum. For thermodynamic equilibrium properties, such as phase stabilities, the spectral function is less clarifying because it enters only after integration over wavevectors and frequencies. To elucidate this issue we computed the vibrational entropy, Svib, in

the harmonic approximation using the phonon density of states obtained from the above-discussed spectral functions (see Figs.S1

throughS4in theSupplemental Information).

Figure 7 shows the results for Svibat 1500 K for the MoTa to

MoTaNbWV and the VW to VWNbTaTi alloy series in (a) and (b), respectively. The black ﬁlled circles and lines represent the full

Fig. 6 Decomposition of the full phonon spectra (ﬁrst column) into contributions of the individual chemical elements (numbers indicate the atomic mass). The projection onto the elements has been performed employing Eqs. (2) and (3). The seemingly weaker contribution of each element when going from top to bottom is a consequence of the reduced concentration of each element in the given alloy i.e. from 50 at.% for the binary (ﬁrst row) to 20 at.% in the bottom row (quinary). Decomposition of the second alloy series (MoTa to MoTaNbWV) is given in theSupplementary Information

calculations including both, mass and force constantﬂuctuations, and the other colored lines represent the various approximations as investigated for the phonon broadening. Interestingly, on an absolute scale, even the virtual-crystal-approximation (VCA; orange lines), i.e., the average over mass and force constant ﬂuctuations, provides a reasonable accuracy, in particular for the MoTa to MoTaNbWV series, with errors of about 0.1 kB. The VCA

error is larger for the other series, reaching up to 0.3 kBfor the VW

binary. The fact that the VW binary shows the largest VCA error can be qualitatively understood with reference to the previous analysis of the spectral function for VW that shows a phonon band gap which cannot be captured by the VCA like phonon dispersion (black line in Fig.1).

Although an error of 0.3 kB may seem small in view of the

absolute vibrational entropy of 8…9 kB at 1500 K, it can become

signiﬁcant when considering competition between phases. Going beyond the VCA approach by including force constantﬂuctuations and averaging only over the masses (blue lines in Figs.7a, b) does not lead to a signiﬁcant improvement. A much better approxima-tion is achieved by including the massﬂuctuations and averaging over the force constants (red lines). This is consistent with our spectral function analysis that the dominating contribution to the phonon broadening is given by the massﬂuctuations.

The dependence of the vibrational entropy on the number of constituents differs for the two alloy series. For the MoTa to MoTaNbWV series the changes are relatively small, while for the VW to VWNbTaTi series the vibrational entropy increases monotonically by a substantial amount from the binary (8.2 kB)

to the quinary (8.9 kB). These dependencies can be, to a good

extent, understood by inspecting the variation of the equilibrium volume and the averaged mass of the alloys, with the volume effect being the dominant one. Generally, increasing the volume results in decreasing phonon frequencies and an enhanced

vibrational entropy, which is responsible for the thermal expan-sion of materials as captured by the quasiharmonic approxima-tion. In this spirit, the strong volume increase when going from VW over to VWNb and then to VWNbTa (blackﬁlled circles and lines in Fig. 7f) is responsible for the signiﬁcant increase in the vibrational entropy for this alloy sequence (blackﬁlled circles and lines in Fig.7b).

The volume effect is modiﬁed by the impact of the atomic masses on the phonon frequencies. With reference to the decomposition performed in Fig. 6 and the corresponding discussion, we note again that light elements, i.e., the ones that decrease the average alloy mass, generally correspond to higher frequency regions and heavier elements, i.e., the ones that tend to increase the average alloy mass, to low frequency regions. The connection to the vibrational entropy is then such that it tends to increase when the average alloy mass decreases. The changes in the average atomic mass can counteract the volume effect (as is the case for VW to VWNb, or the sequence MoTa to MoTaNb to MoTaNbW), or can amplify the volume effect (as for VWNb to VWNbTa). Some additional details of these relationships are given in theSupplementary Information.

Finally, to put the changes observed for the vibrational entropy into a proper perspective, we plot the conﬁgurational entropy (in the ideal approximation) in Figs.7c, d using purposefully the same scale as in Figs.7a, b. The comparison reveals that changes in the vibrational entropy can be of the same magnitude as for the conﬁgurational entropy, and thus we conclude that conﬁgura-tional entropy cannot be a priori assumed to be the single dominating contribution to phase stabilities. This conclusion is further supported by explicitly considering the inﬂuence of ordering, which we have investigated by performing an additional calculation for the B2 (NbTa)(MoW) alloy, reported to be thermodynamically stable at low temperatures.16, 33 This alloy

MoTa **MoTaNb** **MoTaNbW MoTaNbWV**

0.8
1.2
1.6
2
Conf. Entropy (
*k* *B*
)
VW **VWNb** **VWNbTa** **VWNbTaTi**
0.8
1.2
1.6
2

MoTa **MoTaNb** **MoTaNbW MoTaNbWV**

8
8.4
8.8
9.2
Vib. Entropy (
*k* *B*
)
VW **VWNb** **VWNbTa** **VWNbTaTi**
8
8.4
8.8
9.2

Avg. all (VCA) Only mass fluct. Only FC fluct. Full (mass+FC)

MoTa **MoTaNb** **MoTaNbW MoTaNbWV**

16
16.5
17
17.5
18
Volume (Å
3 )
VW **VWNb** **VWNbTa** **VWNbTaTi**
80
100
120
140
160
Mass (u)
VW **VWNb** **VWNbTa** **VWNbTaTi**
15
15.5
16
16.5
17

MoTa **MoTaNb** **MoTaNbW MoTaNbWV**

80 100 120 140 160 ) b ( ) a ( (c) (e) (d) (f)

Binary Ternary Quaternary Quinary Binary Ternary Quaternary Quinary

B2-ordered B2-ordered

Fig. 7 a and b: Vibrational entropy for MoTa to MoTaNbWV and VW to VWNbTaTi at 1500 K derived from the phonon density of states (harmonic approximation). The black solid circles include both mass and force constantﬂuctuations. The orange lines indicate the VCA type spectra (black lines in Fig.1). The red and blue lines represent the vibrational entropy derived from the approximate spectra including either mass or force constantﬂuctuations. The green cross indicates the vibrational entropy derived for a B2 ordered (NbTa)(MoW) alloy (see text for details). c and d show the ideal conﬁgurational entropy of mixing, and e and f the equilibrium volumes (black ﬁlled circles) and averaged atomic masses (greyﬁlled squares) for both alloy series

Phonon broadening in high entropy alloys F Körmann et al.

6

has two sublattices, with one sublattice containing a random distribution of Nb and Ta, and the other sublattice containing a random distribution of Mo and W. Although the ideal con ﬁgura-tional entropy of this alloy is reduced by a factor of 1/2 (green cross in Fig.7c) as compared to the fully disordered A2 NbMoTaW alloy, the computed phonon spectral functions turn out to be very similar (see Fig. S6 in Supplementary Information). This can be understood by the similar mass disorder on each sublattice in the B2 (NbTa)(MoW) as compared to A2 NbMoTaW. As a consequence the derived vibrational entropy (green cross in Fig.7a) is hardly affected. This corroborates the statement that conﬁgurational entropy is not the sole factor in determining phonon broadening and derived thermodynamic properties.

DISCUSSION

The series of ab initio calculations for phonon spectra of refractory high entropy alloys presented here reveals that it is not only the mere number of constituents, which dominates the chemical disorder induced phonon scattering, but rather the inherent ﬂuctuations in the masses and force constants of the elements. For all considered alloys, strong phonon broadening is observed in the range of mid- to high frequencies (above ~ 4 THz). Mass ﬂuctuations dominate the phonon broadening. However, for quantitative predictions force constant ﬂuctuations cannot be neglected. In fact, for some alloys the neglect of force constant ﬂuctuations can result in predictions of artiﬁcial phonon band gaps. In all of the considered alloys the force constantﬂuctuations counteract the mass disorder inducedﬂuctuations. This might be intuited by the fact that we considered elements from the early transition metal series. Qualitatively the relation between atomic mass and force constants can be understood as follows: Increasing the bandﬁlling by going from left to right in the periodic table (e.g. from Hf over Ta to W), not only the atomic masses increase, but also the interatomic bonds are enhanced resulting in increased force constants, which correlates with a decreasing equilibrium volume. Going from top to bottom, e.g. from V over Nb to Ta, the inner core charge and atomic masses increase, resulting in an enhanced local electronic density and thus increased force constants too.

Since atomic mass and force constants jointly contribute to the dynamical matrix and hence phonon energies, this has direct implications for theoretical modeling tools, such as the coherent potential approximation which usually neglect force constant ﬂuctuations.25

The present results further show that conclusions based on a single parameter (e.g. the mass-ﬂuctuation scattering parameter) have little predictive capability because such para-meters can neither fully account for the multi-component element character inherent of high entropy alloys nor account for simultaneous mass and force constantﬂuctuations.

For thermodynamic equilibrium properties, such as the vibra-tional entropy, one may expect that details of the wavevector-resolved spectral functions are of less importance due to the involved integration. Our analysis shows that this expectation is indeed fulﬁlled for the force constant ﬂuctuations that show only a small contribution to the vibrational entropy. In contrast, the integration argument does not work well for the massﬂuctuations which are found to be signiﬁcantly more important. When comparing the vibrational entropy with the conﬁgurational entropy for a varying number of constituents, weﬁnd changes of the same magnitude highlighting the importance of vibrational entropy for phase stability considerations of multicomponent alloys.

For some alloys chemical ordering39has been reported at lower temperatures. This raises the issue in how far chemical ordering affects phonon broadening and vibrational entropies. Since chemical disorder is the key prerequisite for the derived broad-ening one might intuit that it would be strongly suppressed by

any kind of chemical ordering. We ﬁnd, however, that such conclusions do in general not apply for HEAs as our B2 (NbTa) (MoW) example reveals. Even though the partial ordering reduces the conﬁgurational entropy by a factor of 1/2 compared to the fully disordered alloy, almost no impact on the overall phonon broadening and vibrational entropy is found. Based on our analysis we can therefore conclude that it is not the con ﬁgura-tional entropy inherent to HEAs, which controls the vibraﬁgura-tional properties such as broadening or vibrational entropy, but rather the speciﬁc alloy combination of the involved alloy components. The present study is a ﬁrst step towards a full description of lattice excitations in HEAs. Chemical disorder induced scattering is an important part of such a description. The overall phonon broadening at elevated temperatures will be affected by multiple sources (phonon-phonon interactions, extended defect scattering, vacancies). Magnetic ﬂuctuations can be an additional source too.36Alloys featuring multiple-phases40 will give rise to phonon scattering mechanisms on the nanoscale. Recently, an Al-Hf-Sc-Ti-Zr alloy with partial sublattice ordering has been reported.41At the same time recent computer simulations suggest the possibility of selective phonon broadening.42 Noteworthy, the disorder-induced broadened high frequency modes carry the highest energies and therefore constitute a very effective frequency range for such a selective ﬁlter. The combination of computationally engineered materials with designed phonon broadening may open the route towards a new generation of tailored high-temperature HEAs.

METHODS

Electronic structure calculations have been performed with theVASPcode43,44

employing the projector-augmented wave method45_{and the generalized}

gradient approximation.46To ensure high accuracy, the semi-core p-states

of Hf, Mo, Nb, Ta, Ti, V, and W were treated as valence in the employedPAW

potentials. For Zr, semi-core s-states were treated as valence. A plane wave cutoff energy of 400 eV was chosen throughout all calculations. Chemical

disorder was simulated by special quasi random structures (SQS).47 _{The}

SQS have been constructed by minimizing the correlation functions of the ﬁrst two nearest-neighbor shells employing the spcm program. The SQS cells for the equimolar 2-, 3-, 4-, and 5-component alloys contain 128, 54, 128, and 125 atoms. For further informations on the spcm program please contact Prof. Andrei V. Ruban (a.v.ruban@gmail.com) .

The equilibrium volume has been determined by computing total energies for at least nine volumes around the equilibrium volume. The atomic coordinates of each supercell were fully optimized with energy

convergence criteria set to be less than 10−5eV per atom while keeping

the cubic cell shape. The Methfessel-Paxton technique48_{with a smearing}

value of 0.1 eV has been used. For the total energy calculations of the 54-, 125- and 128-atom cells, k-point grids of 6 × 6 × 6, 4 × 4 × 4, and 4 × 4 × 4 (>8000 k-point*atom) have been employed.

The phonon calculations have been performed at the theoretical

equilibrium lattice constant obtained by _{ﬁtting the Vinet equation of}

state49to the total energy calculations. For each alloy, every atom has been

displaced in x-, y-, z-direction by aﬁnite displacement of 0.02 Bohr. To

ensure a high numerical precision, these calculations have been performed

with enhanced energy convergence criteria (<10−7eV) and k-point grids of

7 × 7 × 7 and 5 × 5 × 5 for the 54-atom and 125-, 128-atom cells, respectively (>16,000 k-point*atom). In addition, an additional support grid for the evaluation of the augmentation charges has been employed.

The phonon density of states has been computed employing thePHONOPY

program package.50

The_{ﬁrst-principles derived force constants have been employed in the}

band unfolding method.51–54In this method, phonon spectra of random

alloys are obtained by decomposing the phonon modes of SQS models onto the Brillouin zone of their underlying crystal structures according to their translational symmetry. Pair-projected contributions of the spectral functions are derived by the recently developed mode decomposition

technique37_{and by the proposed modi}

ﬁed projection scheme. A detailed

description is given in theSupplementary Information.

Data availability

The authors declare that all data supporting theﬁndings of this study are

available within the paper and itssupplementary informationﬁles.

ACKNOWLEDGEMENTS

We thank Prof. Andrei V. Ruban for providing the spcm program for generating special quasi-random structures. Discussions with B. Dutta and T. Hickel are acknowledged. Funding by the Deutsche Forschungsgemeinschaft (DFG) through the scholarship KO 5080/1-1, by the European Research Council (ERC) under the European Union’s Horizon 2020 research and innovation programme (Grant agreement No. 639211), by the Ministry of Education, Culture, Sports, Science and Technology (MEXT), Japan, through the Elements Strategy Initiative for Structural Materials (ESISM) of Kyoto University, and by the Japan Society for the Promotion of Science (JSPS) KAKENHI Grant-in-Aid for Young Scientist (B) (Grant No. 16K18228) are gratefully acknowledged.

AUTHOR CONTRIBUTIONS

F.K. and M.S. designed the research, F.K. performed the DFT calculations, Y.I. implemented and applied the band unfolding approach. The results were visualized and analyzed together with B.G. All authors discussed the results and wrote the manuscript.

ADDITIONAL INFORMATION

Supplementary Information accompanies the paper on the npj Computational Materials website (doi:10.1038/s41524-017-0037-8).

Competing interests: The authors declare that they have no competingﬁnancial interests.

Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations.

REFERENCES

1. Gludovatz, B. et al. A fracture-resistant high-entropy alloy for cryogenic applica-tions. Science 345, 1153–1158 (2014).

2. Zou, Y., Ma, H. & Spolenak, R. Ultrastrong ductile and stable high-entropy alloys at small scales. Nat. Commun. 6, 7748 (2015).

3. Kozelj, P. et al. Discovery of a superconducting high-entropy alloy. Phys. Rev. Lett. 113, 107001 (2014).

4. Senkov, O. N., Wilks, G. B., Scott, J. M. & Miracle, D. B. Mechanical properties of Nb25Mo25Ta25W25 and V20Nb20Mo20Ta20W20 refractory high entropy alloys. Intermetallics 19, 698–706 (2011).

5. Senkov, O. N., Wilks, G. B., Miracle, D. B., Chuang, C. P. & Liaw, P. K. Refractory high-entropy alloys. Intermetallics 18, 1758–1765 (2010).

6. Zou, Y., Maiti, S., Steurer, W. & Spolenak, R. Size-dependent plasticity in an Nb25Mo25Ta25W25 refractory high-entropy alloy. Acta. Mater. 65, 85–97 (2014).

7. Lee, J. I., Oh, H. S. & Park, E. S. Manipulation ofσy/κ ratio in single phase FCC solid-solutions. Appl. Phys. Lett. 109, 061906 (2016).

8. Fultz, B. Phase Transitions in Materials. (Cambridge University Press, 2014). 9. Fultz, B. Vibrational thermodynamics of materials. Prog. Mater. Sci. 55, 247–352

(2010).

10. Poudel, B. et al. High-thermoelectric performance of nanostructured bismuth antimony telluride bulk alloys. Science 320, 634–638 (2008).

11. Biswas, K. et al. High-performance bulk thermoelectrics with all-scale hierarchical architectures. Nature. 489, 414–418 (2012).

12. Miracle, D. B. & Senkov, O. N. A critical review of high entropy alloys and related concepts. Acta. Mater. 122, 448–511 (2017).

13. Gao, M. C., Yeh, J.-W., Liaw, P. K. & Zhang, Y. High-Entropy Alloys: Fundamentals and Applications. (Springer, 2016).

14. Murty, B. S., Yeh, J. W. & Ranganathan, S. High-Entropy Alloys. (Butterworth-Hei-nemann, 2014).

15. Oh, H. et al. Lattice distortions in the FeCoNiCrMn high entropy alloy studied by theory and experiment. Entropy 18, 321 (2016).

16. Körmann, F. & Sluiter, M. Interplay between lattice distortions, vibrations and phase stability in NbMoTaW high entropy alloys. Entropy 18, 403 (2016). 17. Wang, W. Y. et al. Revealing the microstates of body-centered-cubic (BCC)

equiatomic high entropy alloys. J. Phase Equilibria Diffus. doi:

10.1007/s11669-017-0565-4(2017).

18. Shafeie, S. et al. High-entropy alloys as high-temperature thermoelectric mate-rials. J. Appl. Phys. 118, 184905 (2015).

19. Fan, Z., Wang, H., Wu, Y., Liu, X. J. & Lu, Z. P. Thermoelectric high-entropy alloys with low lattice thermal conductivity. RSC Adv 6, 52164–52170 (2016). 20. Zhang, Y. et al. Inﬂuence of chemical disorder on energy dissipation and defect

evolution in concentrated solid solution alloys. Nat. Commun. 6, 8736 (2015). 21. Jin, K. et al. Tailoring the physical properties of Ni-based single-phase equiatomic

alloys by modifying the chemical complexity. Sci. Rep 6, 20159 (2016). 22. Dutta, B. & Ghosh, S. Vibrational properties of Ni x Pt 1− x alloys: An

under-standing from ab initio calculations. J. Appl. Phys. 109, 053714 (2011). 23. Grånäs, O., Dutta, B., Ghosh, S. & Sanyal, B. A newﬁrst principles approach to

calculate phonon spectra of disordered alloys. J. Phys. Condens. Matter. 24, 015402 (2011).

24. Dutta, B., Bisht, K. & Ghosh, S. Ab initio calculation of phonon dispersions in size-mismatched disordered alloys. Phys. Rev. B 82, 134207 (2010).

25. Alam, A., Ghosh, S. & Mookerjee, A. Phonons in disordered alloys: Comparison between augmented-space-based approximations for conﬁguration averaging to integration fromﬁrst principles. Phys. Rev. B 75, 134202 (2007).

26. Chouhan, R. K., Alam, A., Ghosh, S. & Mookerjee, A. Interplay of force constants in the lattice dynamics of disordered alloys: Anab initiostudy. Phys. Rev. B 89, 060201(R) (2014).

27. Wang, Y., Zacherl, C. L., Shang, S., Chen, L. Q. & Liu, Z. K. Phonon dispersions in random alloys: a method based on special quasi-random structure force con-stants. J. Phys. Condens. Matter. 23, 485403 (2011).

28. Widom, M. in High-Entropy Alloys: Fundamentals and Applications Ch. 8, (Springer, 2016).

29. Ma, D., Grabowski, B., Körmann, F., Neugebauer, J. & Raabe, D. Ab initio ther-modynamics of the CoCrFeMnNi high entropy alloy: Importance of entropy contributions beyond the conﬁgurational one. Acta. Mater. 100, 90–97 (2015). 30. Song, H., Tian, F. & Wang, D. Thermodynamic properties of refractory high

entropy alloys. J. Alloys Compd. 682, 773–777 (2016).

31. Caro, M., Béland, L. K., Samolyuk, G. D., Stoller, R. E. & Caro, A. Lattice thermal conductivity of multi-component alloys. J. Alloys Compd. 648, 408–413 (2015). 32. Yao, H. W. et al. NbTaV-(Ti,W) refractory high-entropy alloys: Experiments and

modeling. Mater. Sci. Eng., A 674, 203–211 (2016).

33. Körmann, F., Ruban, A. V. & Sluiter, M. H. F. Long-ranged interactions in bcc NbMoTaW high-entropy alloys. Mater. Res. Lett 5, 35–40 (2017).

34. Zhang, Z. et al. Nanoscale origins of the damage tolerance of the high-entropy alloy CrMnFeCoNi. Nat. Commun. 6, 10143 (2015).

35. Klemens, P. G. The scattering of low-frequency lattice waves by static imper-fections. Proc. R. Soc. London, Ser. A 68, 1113 (1955).

36. Ikeda, Y. et al. Temperature-dependent phonon spectra of magnetic random solid solutions. ArXiv e-prints 1702 (2017). http://adsabs.harvard.edu/abs/

2017arXiv170202389I.

37. Ikeda, Y., Carreras, A., Seko, A., Togo, A. & Tanaka, I. Mode decomposition based on crystallographic symmetry in the band-unfolding method. Phys. Rev. B 95, 024305 (2017).

38. Juan, C.-C. et al. Enhanced mechanical properties of HfMoTaTiZr and HfMoNb-TaTiZr refractory high-entropy alloys. Intermetallics 62, 76–83 (2015).

39. Widom, M. Entropy and diffuse scattering: Comparison of NbTiVZr and CrMoNbV. Metallurgical and Materials Transactions A47, 3306–3311 (2016).

40. Li, Z., Pradeep, K. G., Deng, Y., Raabe, D. & Tasan, C. C. Metastable high-entropy dual-phase alloys overcome the strength-ductility trade-off. Nature. 534, 227–230 (2016). 41. Rogal, L. et al. Computational engineering of sublattice ordering in a hexagonal

AlHfScTiZr high entropy alloy. Sci. Rep 7, 2209 (2017).

42. Overy, A. R. et al. Design of crystal-like aperiodic solids with selective disorder-phonon coupling. Nat. Commun. 7, 10445 (2016).

43. Kresse, G. & Furthmüller, J. Efﬁciency of ab-initio total energy calculations for metals and semiconductors using a plane-wave basis set. Comp. Mater. Sci 6, 15–50 (1996).

44. Kresse, G. & Furthmüller, J. Efﬁcient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys. Rev. B 54, 11169–11186 (1996). 45. Blöchl, P. E. Projector augmented-wave method. Phys. Rev. B 50, 17953–17979

(1994).

46. Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865–3868 (1996).

47. Zunger, A., Wei, S., Ferreira, L. G. & Bernard, J. E. Special quasirandom structures. Phys. Rev. Lett. 65, 353–356 (1990).

48. Methfessel, M. & Paxton, A. T. High-precision sampling for Brillouin-zone inte-gration in metals. Phys. Rev. B 40, 3616–3621 (1989).

49. Vinet, P., Ferrante, J., Rose, J. H. & Smith, J. R. J. Geophys. Res. [Solid Earth Planets] 92, 9319 (1987).

50. Togo, A. & Tanaka, I. First principles phonon calculations in materials science. Scripta Mater. 108, 1–5 (2015).

51. Boykin, T. B., Kharche, N., Klimeck, G. & Korkusinski, M. Approximate band-structures of semiconductor alloys from tight-binding supercell calculations. J. Phys. Condens. Matter. 19, 036203 (2007).

Phonon broadening in high entropy alloys F Körmann et al.

8

52. Ku, W., Berlijn, T. & Lee, C. C. Unfoldingﬁrst-principles band structures. Phys. Rev. Lett. 104, 216401 (2010).

53. Popescu, V. & Zunger, A. Extracting E versus k effective band structure from supercell calculations on alloys and impurities. Phys. Rev. B 85, 085201 (2012). 54. Allen, P. B., Berlijn, T., Casavant, D. A. & Soler, J. M. Recovering hidden Bloch

character: Unfolding electrons, phonons, and slabs. Phys. Rev. B 87, 085322 (2013).

Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give

appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visithttp://creativecommons.

org/licenses/by/4.0/.

© The Author(s) 2017